FAILURE OF LVL IN CRUSHING
5. Short-term connection push-out test
5.1 Connection push-out test setup
The connection push-out test setup which was performed in the Structures Laboratory of the Department of Civil and Natural Resources Engineering, University of Canterbury is illustrated in Fig. 3-6 (in main text) and described in Section 4.4 (in main text). 50 mm potentiometers with ±0.4% accuracy: P1, P2, P5 and P6 (Fig. A5-1(a and b)) were used to measure relative slips in connection potentiometer P3 for horizontal slip (Fig. 3-6 in main text). Horizontal slip was measured to observe possible separation between LVL and concrete and to aid in determining whether there would be a problem with the flanges of the specimens separating from the LVL web and falling out, possibly damaging equipment or injuring someone. One specimen was tested without any form of restraint, and it was found that significant separation occurred due to the bending moment induced in the specimen by the load. Since in the actual timber-concrete composite beam the connections are loaded in pure shear and separation between the concrete and timber is not likely to occur, it was decided to prevent the separation in the specimens using steel straps. These were placed at the top and bottom of the specimens for two tests and then the bottom strap only was used for another two tests. It was found that the strength values were almost identical for having two restraints or only one restraint at the bottom; therefore it was decided to just use the single strap at the bottom of the specimens for the rest of the testing.
A potentiometer was used at location P4 (Fig. 3-6 in main text) to compare the difference between measuring the slip at the connection or at the base. This was because previous push-out tests performed by Kuhlmann and Michelfelder (2004) used this form of measurement, and comparison between the results obtained at the connection level and at the base plate will give an indication of the accuracy of this method. No significant
Fig. A5-1. Setting up of push-out test under a Universal Testing Machine: (a) 50 mm potentiometer used to measure relative slip; (b) 20 mm thick steel plate on top of LVL for distribution of load; (c) Specimen slid under loading ram ready for test.
Fig. A5-2. (a) Loading procedure and (b) idealised load-slip curve
All the instrumentation such as the load cells, data acquisition boxes and potentiometers were first calibrated to ensure accuracy in the data recorded. For instance, a scale factor was found for each of the calibrated potentiometers. This scale factor was multiplied by a coefficient measured in the calibration to return the correct measured displacement. A text file containing all the specified channels and corresponding scale factors was written and uploaded into a software known as Universal Data Logger (UDL). This UDL software was used to record the load-relative slip relationships for every channel of each test. Similarly, the load cell which is inherent in the Universal Testing Machine was calibrated as such to
(a) (c) (b)
synchronize the digital read out in the UDL software with the original analog read out of the Universal Testing Machine.
Each specimen which weighed between 100 to 150 kg was positioned on a specially made test platform with the assistance of an overhead crane. The test platform made from steel was placed on the rail of the Universal Testing Machine outside the loading ram. The specimen was seated as such that only the concrete flanges of the specimen were supported and not together with the plywood section. A 20 mm thick steel plate was placed on top of the LVL web to facilitate an even distribution of the load (Fig. A5-1(b)). The length of this plate was made to be the distance between the bottom edges of the two opposite notches cut in the LVL and the width of the plate equal to the width of the LVL piece. Once all the potentiometers have been mounted and the specimen placed correctly, the test platform with the specimen on it was slid carefully under the loading ram of the Universal Testing Machine (Fig. A5-1(c)). A stopper knob was inbuilt onto the test platform so that when the platform is slid under the ram, it would stop in the centre position automatically and any eccentricity eliminated.
The connections were loaded at a rate of 0.2Fest kN per minute in shear with the load
applied onto the LVL web section of the specimen until the connection failed. The load regime followed for the testing is presented in Fig. A5-2(a) as given in EN 26891 (CEN,
1991). This involves an initial estimate of the strength (Fest) of the specimen which was
determined on the basis of experience, preliminary tests, or calculation. This was then
adjusted for the second specimen using the new actual Fest from the first tested specimen.
The specimen was first loaded to 0.4Fest and held for 30 seconds, then unloaded to 0.1Fest
and maintained for 30 seconds. Thereafter the specimen was loaded to failure or to a maximum slip of 20 mm, whichever occurred first.
The purpose of the initial load-unload phase was to eliminate any internal friction in the connection, and to ensure any initial slip or slack present in the connection does not affect the final results. The slip measurements ν01, ν04, ν14, ν11, ν21, ν24, ν26 and ν28 shown in Fig.
A5-2(b) were recorded for each test specimen using potentiometers that were mounted
A2: Rectangular notch 50×50×63
Coach Screw φ16 100 40 10 0.040
A3: Rectangular notch 150×25×63
Coach Screw φ16 130 52 13 0.052
B1: Rectangular notch 150×50×63 100 40 10 0.040
C1: Rectangular notch 150×50×63
Coach Screw φ12 150 60 15 0.060
C2: Rectangular notch 150×50×63
Coach Screw φ16 depth 140 180 72 18 0.072
D1: Doves tail notch 150×50×63 100 40 10 0.040
E1: Triangular notch 30°_60° 137×60×63 100 40 10 0.040
E2: Triangular notch 30°_60° 137×60×63
Coach Screw φ16 150 60 15 0.060
F1: Rectangular notch short end 150×50×63
Coach Screw φ16 150 60 15 0.060
G1: Rectangular notch LSC 150×50×63
Coach Screw φ16 140 56 14 0.056
H1: Rectangular notch double LVL
150×50×126 Coach Screw φ16 260 104 26 0.104
H2: Double toothed mp 650 mm 300 120 30 0.120
H3: Double toothed mp 325 mm 200 80 20 0.080
H4: Double toothed mp 150 mm 100 40 10 0.040
Connections tested in Phase 2:
TT: Triangular notch 30°_60° 137×60×63
Coach Screw φ16, in the weak direction 138 55 14 0.055
T: Triangular notch 30°_60° 137×60×63
Coach Screw φ16, in the strong direction 165 66 16.5 0.066
R: Rectangular notch 300×50×63
Coach Screw φ16 240 112 28 0.112
The load range set on the Universal Testing Machine was 500 kN and therefore the loading rate adjusted on the machine was calculated in kN/min as
500 F 2 . 0 est . Table A5-1 summarizes the types of connection tested with their respective initial estimate of strength
for a pair of connections, Fest, in the loading rate computation.
Fig. A5-3. Load-relative slip of push-out test plotted automatically in the UDL software interface